#------------------------------------------------------------------------------
#$Date: 2016-03-24 03:08:50 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179615 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/79/4507955.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4507955
loop_
_publ_author_name
'Wei, Jingjing'
'Yang, Lu'
'Ma, Pengtao'
'Wang, Jingping'
'Niu, Jingyang'
_publ_section_title
;
 A Series of Multi-Dimensional Lanthanide-Containing
 Peroxoisopolymolybdates
;
_journal_issue                   8
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              3554
_journal_paper_doi               10.1021/cg400536e
_journal_volume                  13
_journal_year                    2013
_chemical_formula_sum            'H115 Mo29 N3 Na2 O158 Pr6'
_chemical_formula_weight         6359.63
_chemical_name_systematic
;

 ?

;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   notdet
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 123.894(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   37.099(7)
_cell_length_b                   16.710(3)
_cell_length_c                   28.416(9)
_cell_measurement_reflns_used    9945
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.10
_cell_measurement_theta_min      2.33
_cell_volume                     14622(6)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0407
_diffrn_reflns_av_sigmaI/netI    0.0479
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -44
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       33
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            36804
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.82
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    4.484
_exptl_absorpt_correction_T_max  0.5161
_exptl_absorpt_correction_T_min  0.2878
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.888
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             11964
_exptl_crystal_size_max          0.37
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.17
_refine_diff_density_max         1.620
_refine_diff_density_min         -0.869
_refine_diff_density_rms         0.205
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.067
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     956
_refine_ls_number_reflns         12809
_refine_ls_number_restraints     72
_refine_ls_restrained_S_all      1.075
_refine_ls_R_factor_all          0.0508
_refine_ls_R_factor_gt           0.0372
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0482P)²+122.2964P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0975
_refine_ls_wR_factor_ref         0.1030
_reflns_number_gt                10420
_reflns_number_total             12809
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg400536e_si_002.cif
_cod_data_source_block           2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               4507955
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Pr1 Pr 0.091461(14) 0.67272(3) 0.365482(18) 0.01673(11) Uani 1 1 d .
Pr2 Pr 0.003396(14) 0.99217(3) 0.362872(18) 0.01571(11) Uani 1 1 d .
Pr3 Pr 0.252520(15) 1.20085(3) 0.30719(2) 0.02328(12) Uani 1 1 d .
Mo1 Mo -0.03402(2) 0.61444(4) 0.30318(3) 0.01548(15) Uani 1 1 d .
Mo2 Mo -0.09456(2) 0.47310(4) 0.29692(3) 0.02100(17) Uani 1 1 d .
Mo3 Mo -0.15438(2) 0.61915(4) 0.28515(3) 0.02064(17) Uani 1 1 d .
Mo4 Mo -0.05259(2) 0.59720(4) 0.40830(3) 0.01750(16) Uani 1 1 d .
Mo5 Mo 0.00533(2) 0.75183(4) 0.40167(3) 0.01570(15) Uani 1 1 d .
Mo6 Mo -0.02118(3) 0.75875(4) 0.49083(3) 0.02281(17) Uani 1 1 d .
Mo7 Mo -0.11809(2) 0.75953(4) 0.38101(3) 0.02290(17) Uani 1 1 d .
Mo8 Mo 0.07940(2) 1.04924(4) 0.30551(3) 0.01516(15) Uani 1 1 d .
Mo9 Mo 0.13710(2) 1.19145(4) 0.30351(3) 0.02101(17) Uani 1 1 d .
Mo10 Mo 0.18658(2) 1.03866(4) 0.29567(3) 0.01958(16) Uani 1 1 d .
Mo11 Mo 0.18623(2) 1.06764(4) 0.41561(3) 0.01798(16) Uani 1 1 d .
Mo12 Mo 0.12140(2) 0.91297(4) 0.40450(3) 0.01547(15) Uani 1 1 d .
Mo13 Mo 0.22228(2) 0.90875(5) 0.50129(3) 0.02427(18) Uani 1 1 d .
Mo14 Mo 0.23258(2) 0.90390(4) 0.39609(3) 0.02214(17) Uani 1 1 d .
Mo15 Mo 0.0000 0.83211(5) 0.2500 0.0138(2) Uani 1 2 d S
Na1 Na 0.10341(14) 0.8304(2) 0.25258(18) 0.0464(10) Uani 1 1 d .
O1 O 0.01841(18) 0.6126(3) 0.3183(2) 0.0247(13) Uani 1 1 d .
O2 O -0.06865(18) 0.6222(3) 0.2303(2) 0.0205(12) Uani 1 1 d .
O3 O -0.03683(18) 0.5014(3) 0.3138(2) 0.0213(13) Uani 1 1 d .
O4 O -0.03486(17) 0.7246(3) 0.3222(2) 0.0181(12) Uani 1 1 d .
O5 O -0.00812(17) 0.6192(3) 0.3967(2) 0.0166(12) Uani 1 1 d .
O6 O -0.08778(17) 0.5947(3) 0.3117(2) 0.0173(12) Uani 1 1 d .
O7 O -0.1210(2) 0.4698(4) 0.2254(2) 0.0317(15) Uani 1 1 d .
O8 O -0.0660(3) 0.3701(4) 0.3224(3) 0.0462(19) Uani 1 1 d .
O9 O -0.1060(2) 0.3712(4) 0.3159(3) 0.0444(18) Uani 1 1 d .
O10 O -0.14537(18) 0.5055(3) 0.2979(2) 0.0233(13) Uani 1 1 d .
O11 O -0.0574(2) 0.4936(3) 0.3986(2) 0.0282(14) Uani 1 1 d .
O12 O -0.1736(2) 0.6244(4) 0.2150(2) 0.0313(15) Uani 1 1 d .
O13 O -0.19996(19) 0.6258(4) 0.2881(3) 0.0299(15) Uani 1 1 d .
O14 O -0.13558(18) 0.7299(3) 0.3043(2) 0.0229(13) Uani 1 1 d .
O15 O -0.11001(18) 0.6267(3) 0.3810(2) 0.0208(13) Uani 1 1 d .
O16 O -0.0267(2) 0.6150(4) 0.4803(2) 0.0286(14) Uani 1 1 d .
O17 O -0.05116(17) 0.7339(3) 0.4064(2) 0.0191(12) Uani 1 1 d .
O18 O 0.05357(18) 0.7333(3) 0.4064(2) 0.0233(13) Uani 1 1 d .
O19 O -0.00159(19) 0.8548(3) 0.3947(2) 0.0226(13) Uani 1 1 d .
O20 O 0.02652(18) 0.7390(3) 0.4797(2) 0.0215(13) Uani 1 1 d .
O21 O -0.0196(2) 0.8603(4) 0.4905(3) 0.0322(15) Uani 1 1 d .
O22 O 0.0248(3) 0.7312(5) 0.5674(3) 0.053(2) Uani 1 1 d .
O23 O -0.0145(3) 0.7357(5) 0.5620(3) 0.053(2) Uani 1 1 d .
O24 O -0.0828(2) 0.7475(4) 0.4619(3) 0.0308(15) Uani 1 1 d .
O25 O -0.1127(2) 0.8596(4) 0.3738(3) 0.0342(16) Uani 1 1 d .
O26 O -0.1680(2) 0.7476(4) 0.3714(3) 0.0315(15) Uani 1 1 d .
O27 O 0.03769(17) 1.0498(3) 0.3159(2) 0.0214(13) Uani 1 1 d .
O28 O 0.05503(17) 1.0410(3) 0.2329(2) 0.0203(12) Uani 1 1 d .
O29 O 0.09106(17) 1.1632(3) 0.3155(2) 0.0222(13) Uani 1 1 d .
O30 O 0.09701(17) 0.9387(3) 0.3253(2) 0.0159(12) Uani 1 1 d .
O31 O 0.13069(17) 1.0456(3) 0.3991(2) 0.0190(12) Uani 1 1 d .
O32 O 0.14277(17) 1.0688(3) 0.3182(2) 0.0176(12) Uani 1 1 d .
O33 O 0.10486(19) 1.1956(4) 0.2325(3) 0.0309(15) Uani 1 1 d .
O34 O 0.1286(2) 1.2940(4) 0.3269(3) 0.052(2) Uani 1 1 d .
O35 O 0.1643(3) 1.2946(4) 0.3239(3) 0.0479(19) Uani 1 1 d .
O36 O 0.19028(18) 1.1583(3) 0.3081(2) 0.0241(13) Uani 1 1 d .
O37 O 0.18352(19) 1.1705(3) 0.4044(2) 0.0267(14) Uani 1 1 d .
O38 O 0.14779(19) 1.0337(4) 0.2245(2) 0.0306(15) Uani 1 1 d .
O39 O 0.23573(19) 1.0485(4) 0.3019(3) 0.0281(14) Uani 1 1 d .
O40 O 0.18648(18) 0.9316(3) 0.3162(2) 0.0240(13) Uani 1 1 d .
O41 O 0.22386(17) 1.0362(3) 0.3932(2) 0.0200(12) Uani 1 1 d .
O42 O 0.21941(19) 1.0528(4) 0.4889(2) 0.0295(15) Uani 1 1 d .
O43 O 0.18395(16) 0.9310(3) 0.4155(2) 0.0182(12) Uani 1 1 d .
O44 O 0.07547(17) 0.9312(3) 0.4051(2) 0.0224(13) Uani 1 1 d .
O45 O 0.12380(18) 0.8098(3) 0.3995(2) 0.0221(13) Uani 1 1 d .
O46 O 0.16348(18) 0.9287(3) 0.4833(2) 0.0218(13) Uani 1 1 d .
O47 O 0.2200(2) 0.8088(4) 0.5022(3) 0.0354(16) Uani 1 1 d .
O48 O 0.2375(3) 0.9377(5) 0.5763(3) 0.055(2) Uani 1 1 d .
O49 O 0.2754(2) 0.9314(5) 0.5739(3) 0.056(2) Uani 1 1 d .
O50 O 0.26340(18) 0.9170(4) 0.4770(2) 0.0294(15) Uani 1 1 d .
O51 O 0.2199(2) 0.8040(4) 0.3879(3) 0.0363(16) Uani 1 1 d .
O52 O 0.2770(2) 0.9117(4) 0.3926(3) 0.0371(16) Uani 1 1 d .
O53 O 0.04593(18) 0.7714(3) 0.2940(2) 0.0212(13) Uani 1 1 d .
O54 O -0.01043(18) 0.8924(3) 0.2919(2) 0.0220(13) Uani 1 1 d .
N1 N 0.1729(3) 0.4608(7) 0.4732(4) 0.083(4) Uani 1 1 d .
N2 N -0.0226(6) 0.2790(13) 0.2824(9) 0.058(6) Uani 0.50 1 d P
O1W O 0.1476(2) 0.7070(4) 0.3447(3) 0.0404(17) Uani 1 1 d .
O2W O 0.1621(2) 0.6727(4) 0.4626(3) 0.049(2) Uani 1 1 d .
O3W O 0.1235(3) 0.5376(4) 0.3689(3) 0.056(2) Uani 1 1 d .
O4W O 0.0882(3) 0.5718(5) 0.4343(4) 0.072(3) Uani 1 1 d .
O5W O 0.0619(2) 1.0957(4) 0.4302(3) 0.0476(19) Uani 1 1 d .
O6W O -0.0266(2) 1.1277(4) 0.3646(3) 0.049(2) Uani 1 1 d .
O7W O -0.0702(2) 0.9590(4) 0.3413(3) 0.051(2) Uani 1 1 d .
O8W O 0.0210(3) 0.9897(4) 0.4632(3) 0.047(2) Uani 1 1 d .
O9W O 0.2867(2) 1.1425(4) 0.4045(3) 0.0457(19) Uani 1 1 d .
O10W O 0.2059(2) 1.1572(5) 0.2037(3) 0.0484(19) Uani 1 1 d .
O11W O 0.2724(2) 1.2995(5) 0.2548(3) 0.055(2) Uani 1 1 d .
O12W O 0.1938(2) 1.3047(4) 0.2501(3) 0.0465(19) Uani 1 1 d .
O13W O 0.2610(2) 1.3141(5) 0.3707(3) 0.060(2) Uani 1 1 d .
O14W O 0.0253(2) 0.4309(4) 0.4194(3) 0.0402(17) Uani 1 1 d U
O15W O 0.0902(3) 0.6467(5) 0.5741(3) 0.035(2) Uani 1 1 d .
O16W O 0.7843(3) 0.4537(4) 0.1655(4) 0.065(3) Uani 1 1 d .
O17W O 0.2262(3) 0.8003(5) 0.6276(4) 0.068(2) Uani 1 1 d .
O18W O 0.0650(5) 1.2374(7) 0.3778(6) 0.040(3) Uani 0.50 1 d PU
O19W O 0.2360(5) 0.9605(8) 0.2155(6) 0.042(3) Uani 0.50 1 d PU
O20W O 0.2130(5) 1.3354(9) 0.4420(6) 0.052(4) Uani 0.50 1 d PU
O21W O 0.3224(4) 0.8955(8) 0.3376(5) 0.123(5) Uani 1 1 d .
O22W O -0.1555(6) 0.9927(9) 0.3824(7) 0.060(5) Uani 0.50 1 d P
O23W O 0.1394(5) 1.2583(12) 0.0418(6) 0.065(5) Uani 0.50 1 d P
O24W O 0.0000 0.4348(16) 0.2500 0.078(8) Uani 0.50 2 d SPU
O25W O 0.0814(8) 0.6199(14) 0.5477(10) 0.077(7) Uani 0.50 1 d PU
O26W O 0.1521(6) 1.0782(11) 0.5279(7) 0.071(5) Uani 0.50 1 d PU
O27W O -0.1117(8) 0.6457(16) 0.5089(11) 0.119(8) Uani 0.50 1 d PU
O28W O 0.0973(7) 1.1174(12) 0.0333(8) 0.098(7) Uani 0.50 1 d PU
O29W O -0.1353(10) 0.510(2) 0.4427(14) 0.158(11) Uani 0.50 1 d PU
O30W O 0.2518(8) 1.2846(14) 0.4634(9) 0.105(7) Uani 0.50 1 d PU
O31W O 0.1188(3) 1.1987(9) 0.1367(4) 0.118(5) Uani 1 1 d .
O32W O -0.0504(13) 0.417(2) 0.1646(17) 0.084(12) Uani 0.25 1 d PU
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pr Pr -0.2180 2.8214 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O53 Pr1 O1 77.36(19) . .
O53 Pr1 O18 78.68(18) . .
O1 Pr1 O18 71.57(19) . .
O53 Pr1 O2 70.29(18) . 2
O1 Pr1 O2 70.70(19) . 2
O18 Pr1 O2 135.20(18) . 2
O53 Pr1 O45 70.30(18) . .
O1 Pr1 O45 136.30(19) . .
O18 Pr1 O45 73.86(19) . .
O2 Pr1 O45 121.66(18) 2 .
O53 Pr1 O1W 86.0(2) . .
O1 Pr1 O1W 139.8(2) . .
O18 Pr1 O1W 140.51(19) . .
O2 Pr1 O1W 69.3(2) 2 .
O45 Pr1 O1W 66.7(2) . .
O53 Pr1 O3W 137.1(2) . .
O1 Pr1 O3W 90.5(2) . .
O18 Pr1 O3W 136.2(2) . .
O2 Pr1 O3W 66.90(19) 2 .
O45 Pr1 O3W 133.2(2) . .
O1W Pr1 O3W 77.3(3) . .
O53 Pr1 O2W 136.6(2) . .
O1 Pr1 O2W 138.3(2) . .
O18 Pr1 O2W 90.1(2) . .
O2 Pr1 O2W 134.5(2) 2 .
O45 Pr1 O2W 66.4(2) . .
O1W Pr1 O2W 76.5(3) . .
O3W Pr1 O2W 77.2(2) . .
O53 Pr1 O4W 139.4(2) . .
O1 Pr1 O4W 69.6(3) . .
O18 Pr1 O4W 69.0(2) . .
O2 Pr1 O4W 117.6(2) 2 .
O45 Pr1 O4W 120.4(2) . .
O1W Pr1 O4W 134.7(3) . .
O3W Pr1 O4W 67.3(3) . .
O2W Pr1 O4W 68.9(3) . .
O54 Pr2 O44 77.90(18) . .
O54 Pr2 O28 70.55(18) . 2
O44 Pr2 O28 135.77(18) . 2
O54 Pr2 O27 75.92(19) . .
O44 Pr2 O27 71.41(18) . .
O28 Pr2 O27 71.41(18) 2 .
O54 Pr2 O7W 87.0(2) . .
O44 Pr2 O7W 140.2(2) . .
O28 Pr2 O7W 68.8(2) 2 .
O27 Pr2 O7W 140.0(2) . .
O54 Pr2 O19 69.47(18) . .
O44 Pr2 O19 73.97(19) . .
O28 Pr2 O19 119.97(18) 2 .
O27 Pr2 O19 135.04(19) . .
O7W Pr2 O19 66.2(2) . .
O54 Pr2 O6W 137.21(19) . .
O44 Pr2 O6W 136.9(2) . .
O28 Pr2 O6W 66.67(19) 2 .
O27 Pr2 O6W 91.5(2) . .
O7W Pr2 O6W 76.8(3) . .
O19 Pr2 O6W 133.5(2) . .
O54 Pr2 O8W 136.0(2) . .
O44 Pr2 O8W 85.2(2) . .
O28 Pr2 O8W 138.9(2) 2 .
O27 Pr2 O8W 135.8(2) . .
O7W Pr2 O8W 80.5(3) . .
O19 Pr2 O8W 66.84(19) . .
O6W Pr2 O8W 80.4(2) . .
O54 Pr2 O5W 140.3(2) . .
O44 Pr2 O5W 71.5(2) . .
O28 Pr2 O5W 116.6(2) 2 .
O27 Pr2 O5W 70.8(2) . .
O7W Pr2 O5W 132.6(3) . .
O19 Pr2 O5W 122.9(2) . .
O6W Pr2 O5W 65.5(2) . .
O8W Pr2 O5W 66.3(2) . .
O36 Pr3 O13 130.99(19) . 3
O36 Pr3 O13W 87.3(2) . .
O13 Pr3 O13W 136.5(2) 3 .
O36 Pr3 O9W 76.9(2) . .
O13 Pr3 O9W 93.5(2) 3 .
O13W Pr3 O9W 73.5(3) . .
O36 Pr3 O12W 74.0(2) . .
O13 Pr3 O12W 132.3(2) 3 .
O13W Pr3 O12W 70.3(2) . .
O9W Pr3 O12W 134.0(3) . .
O36 Pr3 O10W 83.7(2) . .
O13 Pr3 O10W 73.1(2) 3 .
O13W Pr3 O10W 141.0(2) . .
O9W Pr3 O10W 139.5(2) . .
O12W Pr3 O10W 70.7(2) . .
O36 Pr3 O26 143.1(2) . 3
O13 Pr3 O26 68.4(2) 3 3
O13W Pr3 O26 68.1(2) . 3
O9W Pr3 O26 70.2(2) . 3
O12W Pr3 O26 118.8(2) . 3
O10W Pr3 O26 132.6(2) . 3
O36 Pr3 O11W 140.3(2) . .
O13 Pr3 O11W 74.3(2) 3 .
O13W Pr3 O11W 88.4(3) . .
O9W Pr3 O11W 138.6(2) . .
O12W Pr3 O11W 67.4(2) . .
O10W Pr3 O11W 75.4(3) . .
O26 Pr3 O11W 68.5(2) 3 .
O36 Pr3 O39 61.11(18) . .
O13 Pr3 O39 70.51(19) 3 .
O13W Pr3 O39 135.1(2) . .
O9W Pr3 O39 69.0(2) . .
O12W Pr3 O39 122.6(2) . .
O10W Pr3 O39 70.5(2) . .
O26 Pr3 O39 118.66(19) 3 .
O11W Pr3 O39 136.4(2) . .
O36 Pr3 Mo10 33.45(13) . .
O13 Pr3 Mo10 97.62(14) 3 .
O13W Pr3 Mo10 116.5(2) . .
O9W Pr3 Mo10 72.70(15) . .
O12W Pr3 Mo10 99.28(17) . .
O10W Pr3 Mo10 71.61(17) . .
O26 Pr3 Mo10 139.13(14) 3 .
O11W Pr3 Mo10 146.91(19) . .
O39 Pr3 Mo10 27.91(13) . .
O2 Mo1 O1 106.2(3) . .
O2 Mo1 O4 98.4(2) . .
O1 Mo1 O4 98.0(3) . .
O2 Mo1 O3 101.1(2) . .
O1 Mo1 O3 95.4(3) . .
O4 Mo1 O3 152.2(2) . .
O2 Mo1 O6 91.7(2) . .
O1 Mo1 O6 160.2(2) . .
O4 Mo1 O6 87.4(2) . .
O3 Mo1 O6 72.5(2) . .
O2 Mo1 O5 161.3(2) . .
O1 Mo1 O5 91.5(2) . .
O4 Mo1 O5 72.6(2) . .
O3 Mo1 O5 82.9(2) . .
O6 Mo1 O5 71.86(19) . .
O2 Mo1 Mo2 87.67(18) . .
O1 Mo1 Mo2 130.83(19) . .
O4 Mo1 Mo2 127.03(16) . .
O3 Mo1 Mo2 35.47(17) . .
O6 Mo1 Mo2 39.71(14) . .
O5 Mo1 Mo2 85.21(13) . .
O7 Mo2 O9 103.9(3) . .
O7 Mo2 O8 104.5(3) . .
O9 Mo2 O8 42.4(3) . .
O7 Mo2 O3 97.0(3) . .
O9 Mo2 O3 122.0(3) . .
O8 Mo2 O3 80.2(3) . .
O7 Mo2 O10 96.2(3) . .
O9 Mo2 O10 82.8(3) . .
O8 Mo2 O10 124.4(3) . .
O3 Mo2 O10 147.7(2) . .
O7 Mo2 O6 101.5(3) . .
O9 Mo2 O6 147.6(3) . .
O8 Mo2 O6 145.1(3) . .
O3 Mo2 O6 73.9(2) . .
O10 Mo2 O6 74.7(2) . .
O7 Mo2 O11 173.8(2) . .
O9 Mo2 O11 81.8(3) . .
O8 Mo2 O11 81.4(3) . .
O3 Mo2 O11 81.9(2) . .
O10 Mo2 O11 81.8(2) . .
O6 Mo2 O11 72.3(2) . .
O7 Mo2 Mo3 89.8(2) . .
O9 Mo2 Mo3 117.5(2) . .
O8 Mo2 Mo3 157.3(2) . .
O3 Mo2 Mo3 116.08(15) . .
O10 Mo2 Mo3 34.73(16) . .
O6 Mo2 Mo3 42.75(15) . .
O11 Mo2 Mo3 85.25(14) . .
O7 Mo2 Mo1 90.5(2) . .
O9 Mo2 Mo1 155.0(2) . .
O8 Mo2 Mo1 114.5(2) . .
O3 Mo2 Mo1 34.45(15) . .
O10 Mo2 Mo1 116.31(16) . .
O6 Mo2 Mo1 42.12(15) . .
O11 Mo2 Mo1 85.12(14) . .
Mo3 Mo2 Mo1 82.34(3) . .
O12 Mo3 O13 105.6(3) . .
O12 Mo3 O10 100.7(3) . .
O13 Mo3 O10 97.2(3) . .
O12 Mo3 O14 97.4(3) . .
O13 Mo3 O14 97.6(3) . .
O10 Mo3 O14 152.5(2) . .
O12 Mo3 O6 94.0(3) . .
O13 Mo3 O6 159.6(2) . .
O10 Mo3 O6 72.9(2) . .
O14 Mo3 O6 85.5(2) . .
O12 Mo3 O15 162.2(3) . .
O13 Mo3 O15 90.7(2) . .
O10 Mo3 O15 84.0(2) . .
O14 Mo3 O15 72.8(2) . .
O6 Mo3 O15 70.8(2) . .
O12 Mo3 Mo2 88.6(2) . .
O13 Mo3 Mo2 132.9(2) . .
O10 Mo3 Mo2 35.74(17) . .
O14 Mo3 Mo2 125.36(17) . .
O6 Mo3 Mo2 39.91(13) . .
O15 Mo3 Mo2 85.43(14) . .
O16 Mo4 O11 107.3(3) . .
O16 Mo4 O15 101.3(3) . .
O11 Mo4 O15 101.7(3) . .
O16 Mo4 O5 102.1(3) . .
O11 Mo4 O5 100.8(3) . .
O15 Mo4 O5 140.8(2) . .
O16 Mo4 O17 81.5(2) . .
O11 Mo4 O17 171.3(2) . .
O15 Mo4 O17 76.4(2) . .
O5 Mo4 O17 76.5(2) . .
O16 Mo4 O6 171.1(2) . .
O11 Mo4 O6 81.6(2) . .
O15 Mo4 O6 75.7(2) . .
O5 Mo4 O6 76.4(2) . .
O17 Mo4 O6 89.70(19) . .
O19 Mo5 O18 105.4(3) . .
O19 Mo5 O20 100.6(2) . .
O18 Mo5 O20 98.6(3) . .
O19 Mo5 O4 97.5(2) . .
O18 Mo5 O4 97.9(2) . .
O20 Mo5 O4 151.3(2) . .
O19 Mo5 O17 93.3(2) . .
O18 Mo5 O17 160.8(2) . .
O20 Mo5 O17 72.7(2) . .
O4 Mo5 O17 84.2(2) . .
O19 Mo5 O5 162.3(2) . .
O18 Mo5 O5 90.7(2) . .
O20 Mo5 O5 84.0(2) . .
O4 Mo5 O5 72.4(2) . .
O17 Mo5 O5 71.6(2) . .
O19 Mo5 Mo6 87.91(19) . .
O18 Mo5 Mo6 134.56(19) . .
O20 Mo5 Mo6 35.96(17) . .
O4 Mo5 Mo6 123.73(16) . .
O17 Mo5 Mo6 39.50(14) . .
O5 Mo5 Mo6 85.98(13) . .
O21 Mo6 O22 103.5(3) . .
O21 Mo6 O23 102.7(3) . .
O22 Mo6 O23 41.9(3) . .
O21 Mo6 O24 97.4(3) . .
O22 Mo6 O24 122.8(3) . .
O23 Mo6 O24 81.9(3) . .
O21 Mo6 O20 97.4(3) . .
O22 Mo6 O20 80.5(3) . .
O23 Mo6 O20 121.8(3) . .
O24 Mo6 O20 148.2(2) . .
O21 Mo6 O17 101.1(3) . .
O22 Mo6 O17 146.6(3) . .
O23 Mo6 O17 148.7(3) . .
O24 Mo6 O17 75.2(2) . .
O20 Mo6 O17 74.3(2) . .
O21 Mo6 O16 173.7(2) . .
O22 Mo6 O16 82.1(3) . .
O23 Mo6 O16 83.4(3) . .
O24 Mo6 O16 81.6(2) . .
O20 Mo6 O16 80.6(2) . .
O17 Mo6 O16 72.6(2) . .
O21 Mo6 Mo7 90.8(2) . .
O22 Mo6 Mo7 155.7(2) . .
O23 Mo6 Mo7 116.2(3) . .
O24 Mo6 Mo7 34.35(18) . .
O20 Mo6 Mo7 117.53(16) . .
O17 Mo6 Mo7 43.45(15) . .
O16 Mo6 Mo7 84.91(14) . .
O21 Mo6 Mo5 90.3(2) . .
O22 Mo6 Mo5 114.6(3) . .
O23 Mo6 Mo5 155.1(2) . .
O24 Mo6 Mo5 117.87(17) . .
O20 Mo6 Mo5 34.20(15) . .
O17 Mo6 Mo5 42.97(15) . .
O16 Mo6 Mo5 84.71(14) . .
Mo7 Mo6 Mo5 84.35(4) . .
O25 Mo7 O26 106.4(3) . .
O25 Mo7 O24 101.5(3) . .
O26 Mo7 O24 97.6(3) . .
O25 Mo7 O14 95.8(3) . .
O26 Mo7 O14 97.7(3) . .
O24 Mo7 O14 152.5(2) . .
O25 Mo7 O17 92.4(3) . .
O26 Mo7 O17 160.3(2) . .
O24 Mo7 O17 72.3(2) . .
O14 Mo7 O17 85.9(2) . .
O25 Mo7 O15 160.8(3) . .
O26 Mo7 O15 91.0(2) . .
O24 Mo7 O15 83.9(2) . .
O14 Mo7 O15 73.2(2) . .
O17 Mo7 O15 71.5(2) . .
O25 Mo7 Mo6 88.7(2) . .
O26 Mo7 Mo6 132.8(2) . .
O24 Mo7 Mo6 35.17(18) . .
O14 Mo7 Mo6 125.54(17) . .
O17 Mo7 Mo6 39.63(14) . .
O15 Mo7 Mo6 85.30(14) . .
O27 Mo8 O28 106.3(3) . .
O27 Mo8 O30 98.3(2) . .
O28 Mo8 O30 97.9(2) . .
O27 Mo8 O29 96.7(3) . .
O28 Mo8 O29 100.2(2) . .
O30 Mo8 O29 152.1(2) . .
O27 Mo8 O32 161.6(2) . .
O28 Mo8 O32 90.4(2) . .
O30 Mo8 O32 86.4(2) . .
O29 Mo8 O32 72.5(2) . .
O27 Mo8 O31 92.6(2) . .
O28 Mo8 O31 160.1(2) . .
O30 Mo8 O31 72.8(2) . .
O29 Mo8 O31 83.1(2) . .
O32 Mo8 O31 71.7(2) . .
O27 Mo8 Mo9 131.73(19) . .
O28 Mo8 Mo9 87.02(18) . .
O30 Mo8 Mo9 126.12(16) . .
O29 Mo8 Mo9 35.06(17) . .
O32 Mo8 Mo9 39.78(14) . .
O31 Mo8 Mo9 84.75(14) . .
O33 Mo9 O35 103.2(3) . .
O33 Mo9 O34 103.5(3) . .
O35 Mo9 O34 41.9(3) . .
O33 Mo9 O29 96.5(3) . .
O35 Mo9 O29 121.5(3) . .
O34 Mo9 O29 80.2(3) . .
O33 Mo9 O36 96.1(3) . .
O35 Mo9 O36 83.9(3) . .
O34 Mo9 O36 125.1(3) . .
O29 Mo9 O36 147.8(2) . .
O33 Mo9 O32 102.0(3) . .
O35 Mo9 O32 148.1(3) . .
O34 Mo9 O32 145.6(3) . .
O29 Mo9 O32 74.3(2) . .
O36 Mo9 O32 74.1(2) . .
O33 Mo9 O37 174.0(3) . .
O35 Mo9 O37 82.2(3) . .
O34 Mo9 O37 82.2(3) . .
O29 Mo9 O37 82.7(2) . .
O36 Mo9 O37 81.7(2) . .
O32 Mo9 O37 72.1(2) . .
O33 Mo9 Mo8 91.0(2) . .
O35 Mo9 Mo8 154.4(2) . .
O34 Mo9 Mo8 114.3(2) . .
O29 Mo9 Mo8 34.27(15) . .
O36 Mo9 Mo8 116.09(16) . .
O32 Mo9 Mo8 42.48(14) . .
O37 Mo9 Mo8 85.00(14) . .
O38 Mo10 O39 105.5(3) . .
O38 Mo10 O40 100.1(3) . .
O39 Mo10 O40 104.0(3) . .
O38 Mo10 O36 100.7(3) . .
O39 Mo10 O36 85.6(3) . .
O40 Mo10 O36 153.8(2) . .
O38 Mo10 O32 95.1(3) . .
O39 Mo10 O32 152.5(2) . .
O40 Mo10 O32 89.9(2) . .
O36 Mo10 O32 72.6(2) . .
O38 Mo10 O41 165.0(2) . .
O39 Mo10 O41 89.3(2) . .
O40 Mo10 O41 73.4(2) . .
O36 Mo10 O41 82.6(2) . .
O32 Mo10 O41 71.8(2) . .
O38 Mo10 Pr3 103.2(2) . .
O39 Mo10 Pr3 44.5(2) . .
O40 Mo10 Pr3 145.02(18) . .
O36 Mo10 Pr3 41.50(16) . .
O32 Mo10 Pr3 113.46(14) . .
O41 Mo10 Pr3 88.97(13) . .
O37 Mo11 O42 106.8(3) . .
O37 Mo11 O31 101.8(3) . .
O42 Mo11 O31 102.4(3) . .
O37 Mo11 O41 100.9(3) . .
O42 Mo11 O41 101.5(3) . .
O31 Mo11 O41 140.4(2) . .
O37 Mo11 O43 171.2(2) . .
O42 Mo11 O43 82.0(2) . .
O31 Mo11 O43 76.6(2) . .
O41 Mo11 O43 75.9(2) . .
O37 Mo11 O32 80.9(2) . .
O42 Mo11 O32 172.3(2) . .
O31 Mo11 O32 76.4(2) . .
O41 Mo11 O32 75.6(2) . .
O43 Mo11 O32 90.32(19) . .
O45 Mo12 O44 105.6(3) . .
O45 Mo12 O46 100.8(2) . .
O44 Mo12 O46 97.4(2) . .
O45 Mo12 O30 97.9(2) . .
O44 Mo12 O30 98.4(2) . .
O46 Mo12 O30 151.2(2) . .
O45 Mo12 O43 92.9(2) . .
O44 Mo12 O43 160.6(2) . .
O46 Mo12 O43 72.8(2) . .
O30 Mo12 O43 84.6(2) . .
O45 Mo12 O31 162.0(2) . .
O44 Mo12 O31 90.9(2) . .
O46 Mo12 O31 83.6(2) . .
O30 Mo12 O31 72.3(2) . .
O43 Mo12 O31 71.6(2) . .
O45 Mo12 Mo13 87.67(18) . .
O44 Mo12 Mo13 133.03(19) . .
O46 Mo12 Mo13 35.64(17) . .
O30 Mo12 Mo13 124.67(16) . .
O43 Mo12 Mo13 40.04(14) . .
O31 Mo12 Mo13 85.99(13) . .
O47 Mo13 O49 102.1(3) . .
O47 Mo13 O48 102.5(3) . .
O49 Mo13 O48 43.9(3) . .
O47 Mo13 O46 96.5(3) . .
O49 Mo13 O46 124.4(3) . .
O48 Mo13 O46 81.1(3) . .
O47 Mo13 O50 97.5(3) . .
O49 Mo13 O50 80.5(3) . .
O48 Mo13 O50 123.5(3) . .
O46 Mo13 O50 147.8(2) . .
O47 Mo13 O43 101.1(3) . .
O49 Mo13 O43 147.9(3) . .
O48 Mo13 O43 147.5(3) . .
O46 Mo13 O43 74.3(2) . .
O50 Mo13 O43 74.6(2) . .
O47 Mo13 O42 173.7(3) . .
O49 Mo13 O42 84.1(3) . .
O48 Mo13 O42 82.8(3) . .
O46 Mo13 O42 80.9(2) . .
O50 Mo13 O42 82.0(2) . .
O43 Mo13 O42 72.7(2) . .
O47 Mo13 Mo12 89.4(2) . .
O49 Mo13 Mo12 157.8(3) . .
O48 Mo13 Mo12 115.3(2) . .
O46 Mo13 Mo12 34.22(15) . .
O50 Mo13 Mo12 117.18(16) . .
O43 Mo13 Mo12 43.00(15) . .
O42 Mo13 Mo12 85.24(14) . .
O47 Mo13 Mo14 91.4(2) . .
O49 Mo13 Mo14 114.6(3) . .
O48 Mo13 Mo14 156.2(2) . .
O46 Mo13 Mo14 116.80(16) . .
O50 Mo13 Mo14 34.16(16) . .
O43 Mo13 Mo14 42.77(15) . .
O42 Mo13 Mo14 84.74(14) . .
Mo12 Mo13 Mo14 83.64(3) . .
O52 Mo14 O51 105.5(3) . .
O52 Mo14 O50 96.4(3) . .
O51 Mo14 O50 102.0(3) . .
O52 Mo14 O40 99.1(3) . .
O51 Mo14 O40 94.3(3) . .
O50 Mo14 O40 153.6(2) . .
O52 Mo14 O43 161.3(3) . .
O51 Mo14 O43 91.8(3) . .
O50 Mo14 O43 72.7(2) . .
O40 Mo14 O43 86.3(2) . .
O52 Mo14 O41 92.7(3) . .
O51 Mo14 O41 159.6(3) . .
O50 Mo14 O41 84.8(2) . .
O40 Mo14 O41 73.3(2) . .
O43 Mo14 O41 71.6(2) . .
O52 Mo14 Mo13 132.0(2) . .
O51 Mo14 Mo13 89.1(2) . .
O50 Mo14 Mo13 35.66(18) . .
O40 Mo14 Mo13 125.58(17) . .
O43 Mo14 Mo13 39.32(13) . .
O41 Mo14 Mo13 85.40(14) . .
O54 Mo15 O54 110.2(4) 2 .
O54 Mo15 O53 109.8(3) 2 2
O54 Mo15 O53 108.5(3) . 2
O54 Mo15 O53 108.5(3) 2 .
O54 Mo15 O53 109.8(3) . .
O53 Mo15 O53 109.9(4) 2 .
O4 Na1 O30 122.3(2) 2 .
O4 Na1 O1W 92.9(2) 2 .
O30 Na1 O1W 91.7(2) . .
O4 Na1 O14 73.04(18) 2 2
O30 Na1 O14 164.4(2) . 2
O1W Na1 O14 84.2(2) . 2
Mo1 O1 Pr1 149.6(3) . .
Mo1 O2 Pr1 154.5(3) . 2
Mo1 O3 Mo2 110.1(3) . .
Mo1 O4 Mo5 115.4(3) . .
Mo1 O4 Na1 122.2(2) . 2
Mo5 O4 Na1 120.6(2) . 2
Mo4 O5 Mo5 111.3(2) . .
Mo4 O5 Mo1 110.9(2) . .
Mo5 O5 Mo1 92.42(18) . .
Mo2 O6 Mo1 98.2(2) . .
Mo2 O6 Mo3 97.3(2) . .
Mo1 O6 Mo3 150.4(3) . .
Mo2 O6 Mo4 100.7(2) . .
Mo1 O6 Mo4 100.8(2) . .
Mo3 O6 Mo4 101.0(2) . .
O9 O8 Mo2 67.6(4) . .
O8 O9 Mo2 70.0(4) . .
Mo3 O10 Mo2 109.5(3) . .
Mo4 O11 Mo2 105.5(3) . .
Mo3 O13 Pr3 151.4(3) . 3_445
Mo3 O14 Mo7 113.4(3) . .
Mo3 O14 Na1 124.7(3) . 2
Mo7 O14 Na1 118.2(2) . 2
Mo4 O15 Mo7 112.4(3) . .
Mo4 O15 Mo3 112.1(3) . .
Mo7 O15 Mo3 92.7(2) . .
Mo4 O16 Mo6 105.7(3) . .
Mo6 O17 Mo5 97.5(2) . .
Mo6 O17 Mo7 96.9(2) . .
Mo5 O17 Mo7 153.2(3) . .
Mo6 O17 Mo4 100.3(2) . .
Mo5 O17 Mo4 100.0(2) . .
Mo7 O17 Mo4 99.5(2) . .
Mo5 O18 Pr1 149.2(3) . .
Mo5 O19 Pr2 155.8(3) . .
Mo5 O20 Mo6 109.8(3) . .
O23 O22 Mo6 69.3(5) . .
O22 O23 Mo6 68.8(4) . .
Mo7 O24 Mo6 110.5(3) . .
Mo7 O26 Pr3 148.2(3) . 3_445
Mo8 O27 Pr2 149.4(3) . .
Mo8 O28 Pr2 152.2(3) . 2
Mo8 O29 Mo9 110.7(3) . .
Mo8 O30 Mo12 114.3(3) . .
Mo8 O30 Na1 123.0(2) . .
Mo12 O30 Na1 121.6(2) . .
Mo11 O31 Mo8 112.2(2) . .
Mo11 O31 Mo12 111.3(3) . .
Mo8 O31 Mo12 92.65(19) . .
Mo9 O32 Mo10 100.5(2) . .
Mo9 O32 Mo8 97.7(2) . .
Mo10 O32 Mo8 148.1(3) . .
Mo9 O32 Mo11 100.1(2) . .
Mo10 O32 Mo11 102.8(2) . .
Mo8 O32 Mo11 99.5(2) . .
O35 O34 Mo9 68.6(4) . .
O34 O35 Mo9 69.5(4) . .
Mo9 O36 Mo10 107.3(3) . .
Mo9 O36 Pr3 146.6(3) . .
Mo10 O36 Pr3 105.0(2) . .
Mo11 O37 Mo9 106.9(3) . .
Mo10 O39 Pr3 107.5(3) . .
Mo10 O40 Mo14 115.2(3) . .
Mo11 O41 Mo14 112.3(3) . .
Mo11 O41 Mo10 109.7(2) . .
Mo14 O41 Mo10 92.28(19) . .
Mo11 O42 Mo13 105.0(3) . .
Mo13 O43 Mo12 97.0(2) . .
Mo13 O43 Mo14 97.9(2) . .
Mo12 O43 Mo14 152.6(3) . .
Mo13 O43 Mo11 100.3(2) . .
Mo12 O43 Mo11 100.0(2) . .
Mo14 O43 Mo11 99.8(2) . .
Mo12 O44 Pr2 150.6(3) . .
Mo12 O45 Pr1 154.2(3) . .
Mo12 O46 Mo13 110.1(3) . .
O49 O48 Mo13 68.0(4) . .
O48 O49 Mo13 68.1(4) . .
Mo14 O50 Mo13 110.2(3) . .
Mo15 O53 Pr1 158.5(3) . .
Mo15 O54 Pr2 157.8(3) . .
Pr1 O1W Na1 103.9(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pr1 O53 2.424(5) .
Pr1 O1 2.470(5) .
Pr1 O18 2.486(6) .
Pr1 O2 2.503(5) 2
Pr1 O45 2.515(5) .
Pr1 O1W 2.525(6) .
Pr1 O3W 2.528(7) .
Pr1 O2W 2.534(6) .
Pr1 O4W 2.635(8) .
Pr2 O54 2.441(5) .
Pr2 O44 2.460(5) .
Pr2 O28 2.489(5) 2
Pr2 O27 2.494(5) .
Pr2 O7W 2.504(7) .
Pr2 O19 2.511(5) .
Pr2 O6W 2.535(6) .
Pr2 O8W 2.546(7) .
Pr2 O5W 2.595(7) .
Pr3 O36 2.430(6) .
Pr3 O13 2.458(6) 3
Pr3 O13W 2.510(8) .
Pr3 O9W 2.510(6) .
Pr3 O12W 2.540(7) .
Pr3 O10W 2.549(7) .
Pr3 O26 2.575(6) 3
Pr3 O11W 2.589(7) .
Pr3 O39 2.605(6) .
Pr3 Mo10 3.5416(10) .
Mo1 O2 1.729(5) .
Mo1 O1 1.742(6) .
Mo1 O4 1.923(5) .
Mo1 O3 1.924(5) .
Mo1 O6 2.165(5) .
Mo1 O5 2.268(5) .
Mo1 Mo2 3.1950(11) .
Mo2 O7 1.694(6) .
Mo2 O9 1.906(6) .
Mo2 O8 1.937(7) .
Mo2 O3 1.974(6) .
Mo2 O10 1.976(6) .
Mo2 O6 2.062(5) .
Mo2 O11 2.434(6) .
Mo2 Mo3 3.1884(11) .
Mo3 O12 1.704(6) .
Mo3 O13 1.743(6) .
Mo3 O10 1.927(5) .
Mo3 O14 1.945(6) .
Mo3 O6 2.182(5) .
Mo3 O15 2.269(5) .
Mo4 O16 1.734(6) .
Mo4 O11 1.747(6) .
Mo4 O15 1.882(6) .
Mo4 O5 1.890(5) .
Mo4 O17 2.287(5) .
Mo4 O6 2.289(5) .
Mo5 O19 1.734(5) .
Mo5 O18 1.746(6) .
Mo5 O20 1.906(5) .
Mo5 O4 1.944(5) .
Mo5 O17 2.193(5) .
Mo5 O5 2.259(5) .
Mo5 Mo6 3.1903(13) .
Mo6 O21 1.698(6) .
Mo6 O22 1.928(7) .
Mo6 O23 1.933(7) .
Mo6 O24 1.959(6) .
Mo6 O20 1.992(6) .
Mo6 O17 2.047(5) .
Mo6 O16 2.415(6) .
Mo6 Mo7 3.1861(12) .
Mo7 O25 1.710(6) .
Mo7 O26 1.727(6) .
Mo7 O24 1.919(6) .
Mo7 O14 1.959(6) .
Mo7 O17 2.207(5) .
Mo7 O15 2.239(5) .
Mo8 O27 1.730(5) .
Mo8 O28 1.735(5) .
Mo8 O30 1.935(5) .
Mo8 O29 1.938(5) .
Mo8 O32 2.195(5) .
Mo8 O31 2.248(5) .
Mo8 Mo9 3.2200(10) .
Mo9 O33 1.679(6) .
Mo9 O35 1.917(7) .
Mo9 O34 1.927(7) .
Mo9 O29 1.977(6) .
Mo9 O36 1.982(6) .
Mo9 O32 2.079(5) .
Mo9 O37 2.409(6) .
Mo10 O38 1.710(6) .
Mo10 O39 1.739(6) .
Mo10 O40 1.883(6) .
Mo10 O36 2.022(6) .
Mo10 O32 2.114(5) .
Mo10 O41 2.305(5) .
Mo11 O37 1.741(6) .
Mo11 O42 1.747(6) .
Mo11 O31 1.877(5) .
Mo11 O41 1.904(6) .
Mo11 O43 2.284(5) .
Mo11 O32 2.298(5) .
Mo12 O45 1.737(5) .
Mo12 O44 1.740(5) .
Mo12 O46 1.903(5) .
Mo12 O30 1.948(5) .
Mo12 O43 2.183(5) .
Mo12 O31 2.261(5) .
Mo12 Mo13 3.1774(11) .
Mo13 O47 1.674(6) .
Mo13 O49 1.936(7) .
Mo13 O48 1.938(7) .
Mo13 O46 1.972(6) .
Mo13 O50 1.999(6) .
Mo13 O43 2.059(5) .
Mo13 O42 2.426(6) .
Mo13 Mo14 3.2190(15) .
Mo14 O52 1.709(6) .
Mo14 O51 1.714(6) .
Mo14 O50 1.926(6) .
Mo14 O40 1.991(6) .
Mo14 O43 2.207(5) .
Mo14 O41 2.229(5) .
Mo15 O54 1.759(5) 2
Mo15 O54 1.759(5) .
Mo15 O53 1.766(5) 2
Mo15 O53 1.766(5) .
Na1 O4 2.843(7) 2
Na1 O30 2.856(7) .
Na1 O1W 3.001(9) .
Na1 O14 3.002(7) 2
O2 Pr1 2.503(5) 2
O4 Na1 2.843(7) 2
O8 O9 1.390(10) .
O13 Pr3 2.458(6) 3_445
O14 Na1 3.002(7) 2
O22 O23 1.380(11) .
O26 Pr3 2.575(6) 3_445
O28 Pr2 2.489(5) 2
O34 O35 1.374(10) .
O48 O49 1.449(11) .
O15W O25W 0.77(2) .
O20W O30W 1.48(3) .
